Osmotic Blisters: The Plague of Resin Floors
Since the 1960s, builders and consumers have selected resin floors for their seamless strength. Base resin, when mixed with reactive hardener, induces in situ polymerisation. Although builders use different chemicals to manufacture resin floors, this curing reaction is critical to their formation.
High School Chemistry: Osmosis
When builders apply resin floors to concrete with adhesives, bonding adhesives form a partially-permeable membrane. Think of the concrete as one slice of bread. The synthetic resin floor covering is the other slice, and adhesive holds the sandwich together. During procurement, moisture content (MC) flows from the more diluted solution to the more concentrated one – in this case from concrete to resin. That’s as far as theory can safely be applied to resin floors.
The adhesive membranes cause unequal moisture migration. Put simply, the membrane allows safe passage to MC while denying similar migration to dissolved substances. In essence, MC saturates one slice of bread at the expense of MC in the other.
Osmotic blisters are a building contractor’s nightmare for two reasons. First (and obviously), they can ruin otherwise good work. Secondly, too many builders install resin floors without knowing the profound influence of MC on the formation of osmotic blisters. Any time one element passes more freely than another, imbalance ensues.
Apply resin floors to un-equilibrated concrete substrate slabs, and you invite the MC to blister the surface of resin floors. In order to fix them, we must first understand osmotic blisters.
The Ingredients of Osmotic Blisters
- Semi-permeable membrane: in construction, it is often the bond interface or the extreme upper layer of the concrete.
- Concentrated water-soluble material (organic or inorganic): the wild card. This can be traced to anything from the resin ingredients in the epoxy coating, or concrete admixtures. Soluble salt content in concrete will do it, too.
- Water: one concrete’s three core ingredients. MC always rises from the bottom of the slab to the top to reach compressive strength, concrete’s destination of choice.
The Natural Cure: Moisture Content
There is no litmus test for osmotic blisters. However, relative humidity (RH) measurement provides installers with all-important data on concrete readiness. Equilibrated RH levels are reached when the slab’s RH% is “balanced” with that of its surrounding service temperature and RH. If RH is too high, builders must hold off on the installation of resin floors.
- Try to minimize the amount of soluble salts in the concrete mix design.
- Install a water vapor barrier beneath the slab.
- Avoid acid etching as surface preparation for a coating application.
- Check that the epoxy coating resin constituents are accurately-proportioned and properly mixed.
- Check the slab’s RH during curing and drying to ensure its readiness.
Latest posts by Jason Spangler (see all)
- How to Prepare a Concrete Floor for Coatings - September 14, 2016
- RH Testing and That 72-Hour Wait: How Do You Manage It? - August 9, 2016
- 5 Ways to Speed up Your Concrete Moisture Testing - August 5, 2016